High Mobility, Printable, andSolution-Processed Graphene ElectronicsShuai Wang,,| Priscilla Kailian Ang,,,| Ziqian Wang, Ai Ling Lena Tang,John T. L. Thong, and Kian Ping Loh*,
Department of Chemistry, National University of Singapore, 3 Science Drive 3, Singapore 117543, NUS GraduateSchool for Integrative Sciences and Engineering, Singapore 117597, and Department of Electrical and ComputerEngineering, 4 Engineering Drive 3, Singapore 117576
ABSTRACT The ability to print graphene sheets onto large scale, flexible substrates holds promise for large scale, transparentelectronics on flexible substrates. Solution processable graphene sheets derived from graphite can form stable dispersions in solutionsand are amenable to bulk scale processing and ink jet printing. However, the electrical conductivity and carrier mobilities of thismaterial are usually reported to be orders of magnitude poorer than that of the mechanically cleaved counterpart due to its higherdensity of defects, which restricts its use in electronics. Here, we show that by optimizing several key factors in processing, we areable to fabricate high mobility graphene films derived from large sized graphene oxide sheets, which paves the way for all-carbonpost-CMOS electronics. All-carbon source-drain channel electronics fabricated from such films exhibit significantly improved transportcharacteristics, with carrier mobilities of 365 cm2/(Vs) for hole and 281 cm2/(Vs) for electron, measured in air at room temperature.In particular, intrinsic mobility as high as 5000 cm2/(Vs) can be obtained from such solution-processed graphene films when ionicscreening is applied to nullify the Coulombic scattering by charged impurities.
KEYWORDS Graphene, high mobility transistor, solution-processed, printable electronics, ionic screening, doping, impurityscattering
The discovery of graphene has revolutionized the fieldof electronics owing to its excellent electronic proper-ties and chemical and mechanical stability, whichpaves the way for ultrafast electronic devices and bio- andchemical sensors.1,2 The mechanical exfoliation, or Scotchtape method, has been used to produce the first high-qualitygraphene sheets which set the performance standard forgraphene produced by other methods. However, the Scotchtape method is not compatible with large-scale industrialprocessing and precludes the widespread implementationof graphene electronics; thus there are intense efforts world-wide to discover upwardly scalable production methods forhigh-quality graphene. Recent breakthroughs include thelarge-area deposition of few-layer graphene (FLG) usingchemical vapor deposition on catalyst-coated substrates.3
Another research thrust involves the solution processing ofgraphene derivatives. Chemical exfoliation methods whichproduce graphene oxide from graphite result in high-yieldproduction of single sheet dispersions.4,5 The solution-processability of GO offers unique advantages since it isreadily amenable to spin-coating, spray-casting, drop-cast-ing, or inkjet printing onto substrates for large-scale produc-tion of graphene electronic circuits. The deoxidation ofgraphene oxide (GO) by chemical reduction and thermalannealing has been shown to produce zero-band-gap semi-
metal graphene nanosheets which can exhibit trap-free bandtransport despite defects and disorder.6 However, the tran-sistor carrier mobility in such a GO-derived graphene thinfilm is usually between 0.1 and 1 cm2/(Vs) as reported inliterature,4,6,7 which is several orders lower than that of themechanically cleaved graphene. There are several possibili-ties for the poor performance in these chemically processedgraphene (CPG). The charge percolation is limited by discon-nected network of -delocalized tracks in these CPG. Defectscreated after the removal of C-O functional groups hinderthe full recovery of the charge transport properties of pristinegraphene8 and further processing is needed to recover theextended aromatic framework. Therefore, there are stillsignificant challenges ahead before CPG can be used in highmobility electronic devices.
In this work, we discovered that by optimizing several keyfactors in film processing and device fabrication, unprec-edented performance in the electrical transport propertiesof CPG can be obtained. Our results reaffirm that CPG retainsthe intrinsic structural coherence for high mobility transport.Building upon this, we have also explored the premise ofusing CPG for inkjet printable all-carbon electronics.
For electronic applications, the mobility and conductivityof graphene sheets are critical.8 However it is widely knownthat the electrical characteristics of CPG are generally verypoor. A survey of most reports found that a large percentageof CPG consists of GO flakes with sizes 1 m or less due toprolonged ultrasonication and harsh oxidation treatment ofthe colloidal GO suspension.4-11 We have a simple hypoth-
* Corresponding author, firstname.lastname@example.org.|These authors contributed equally.Received for review: 09/2/2009Published on Web: 12/21/2009
2010 American Chemical Society 92 DOI: 10.1021/nl9028736 | Nano Lett. 2010, 10, 92-98
esis. We propose that the poor electrical characteristics canbe circumvented by using big sized GO (BSGOs) with lateralsize above 25 m. Submicrometer sized GOs synthesizedby harsh oxidation conditions have a higher density ofdefects relative to BSGOs, due to the fact that the generationof smaller sized sheets from larger sized ones involveschemical destruction of aromatic bonds. The density of thesedefects may scale in a nonlinear way with the area of GOs;smaller GOs have a significantly larger density of disorderand defects on the basal planes due to a higher compositionof nonstoichiometric oxygen. Another important implicationin transport measurement is that for an edge-to-edge con-tinuous film constructed from networks of graphene flakes,the larger flakes should give a lower number of sheet-to-sheet junctions compared to the smaller flakes within a fixedchannel length.
Here we report a reproducible and simple method toobtain high-quality BSGO (Figure 1a) where more than 20%of the flakes have lateral dimension larger than 25 m,according to size-counting using optical micrograph andscanning electron microscopy (SEM) images. Our methodis based on the modified Hummers method.7 We appliedcareful gradient separation and minimized the number ofsonication steps to avoid breaking up the larger sized GOsheets. (See Methods in Supporting Information.) Such BSGOsheets possess a significantly reduced number of C-Ogroups compared to small-sized GO, as evident from therelative proportion of the C-C bond versus C-O bonds inthe deconvoluted X-ray photoelectron spectroscopy (XPS)spectra. The deconvoluted area assignable to the C-C bondsof graphene (Figure 1d) is higher than that of small-sized GOby 10%.11 Despite a lower proportion of C-O groups, theaqueous solution of BSGO remains stable and opaque over
several months in concentrations as high as 50 mg mL-1
(Figure 1b). In addition, spin-coating of the BSGO solutiononto a SiO2/Si substrate allows the formation of a uniform,continuous graphene thin film as shown in Figure 1c wherethe film morphology probed by atomic force microscopy(AFM) shows incommensurately stacked BSGO sheets withthe edges of individual GO sheets clearly visible. By varyingthe concentration of BSGO solution, we are able to tune thethickness of the graphene film selectively from one to threelayers. Upon thermal annealing of BSGO-coated SiO2/Sisubstrate at 1000 C, the C 1s peak signal assignable to theC-C bonds of graphene increases from 53% to 89%. AFMmeasurement also indicates a reduction of sheet thicknessfrom 1 nm, due to protruding oxygen groups on either sideof GO sheets, to 0.53 nm, a characteristic thickness ofgraphene sheet (see Figure S3 in Supporting Information).Significant structural changes reflective of the restoration ofdelocalized -conjugation in GO-derived graphene sheets arealso evident from their Raman spectra (Figure 1d). The Gband for reduced BSGO is sharper and shifts to lowerfrequency (1586 cm-1) as compared to BSGO (1594 cm-1).The ratio of Raman D to G band intensity (ID/IG) decreasesfrom 0.81 to 0.78, thus indicating an increase in the averagesize of sp2 domains on reduced BSGO. The restoration of the-conjugated structure in the BSGO sheets translates to ahigh conductivity of 760 S/cm, which is close to that ofpolycrystalline graphite (1250 S/cm) (see Figures S4 and S5in Supporting Information). This makes these graphenesheets an attractive candidate for making continuous, highlyconducting graphene thin films by spin-coating or printingtechnologies amenable to large scale processing.
To investigate the transport characteristics of thesegraphene films, we fabricated graphene thin film field-effect
FIGURE 1. Big-sized GO (BSGO) sheets and their characterization. (a) AFM image of BSGO. (b) The narrow size distribution of BSGOs withGaussian mean at 250 ( 10 m2. (c) AFM image of BSGO films showing good film morphology. Inset: GO solution remains stable after 5months with a concentration as high as 50 mg mL-1. (d) Deconvolution of XPS spectra and Raman spectra for BSGO before and after thermalannealing at 1000 C.
2010 American Chemical Society 93 DOI: 10.1021/nl9028736 | Nano Lett. 2010, 10, 92-98